#------------------------------------------------------------------------------
#$Date: 2016-03-23 00:20:41 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179105 $
#$URL: svn://www.crystallography.net/cod/cif/4/30/67/4306710.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4306710
loop_
_publ_author_name
'Bayrammurad Saparov'
'Sheng-qing Xia'
'Svilen Bobev'
_publ_section_title
;
Synthesis, Structure, and Bonding of the Zintl Phase Ba3Cd2Sb4
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              11237
_journal_page_last               11244
_journal_paper_doi               10.1021/ic801530d
_journal_volume                  47
_journal_year                    2008
_chemical_formula_moiety         '2(Cd Sb2), 3(Ba)'
_chemical_formula_sum            'Ba3 Cd2 Sb4'
_chemical_formula_weight         1123.82
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 112.2140(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   17.8351(16)
_cell_length_b                   4.8675(5)
_cell_length_c                   7.6837(7)
_cell_measurement_reflns_used    711
_cell_measurement_temperature    120(2)
_cell_measurement_theta_max      26.36
_cell_measurement_theta_min      2.47
_cell_volume                     617.53(10)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      120(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0208
_diffrn_reflns_av_sigmaI/netI    0.0169
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_h_min       -22
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            3298
_diffrn_reflns_theta_full        26.36
_diffrn_reflns_theta_max         26.36
_diffrn_reflns_theta_min         2.47
_exptl_absorpt_coefficient_mu    21.307
_exptl_absorpt_correction_T_max  0.5061
_exptl_absorpt_correction_T_min  0.3764
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
; 
SADABS (Sheldrick, 2003) 
;
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    6.044
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             936
_exptl_crystal_size_max          0.06
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.04
_refine_diff_density_max         0.653
_refine_diff_density_min         -1.061
_refine_diff_density_rms         0.254
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.235
_refine_ls_matrix_type           full
_refine_ls_number_parameters     29
_refine_ls_number_reflns         711
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.235
_refine_ls_R_factor_all          0.0177
_refine_ls_R_factor_gt           0.0164
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0188P)²+0.1319P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0393
_refine_ls_wR_factor_ref         0.0397
_reflns_number_gt                683
_reflns_number_total             711
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic801530d_si_002_1.cif
_cod_data_source_block           Ba3Cd2Sb4
_cod_original_sg_symbol_H-M      'C 2/m'
_cod_database_code               4306710
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Ba1 Ba 0.14194(2) 0.0000 0.59031(5) 0.01046(11) Uani 1 2 d S . .
Ba2 Ba 0.0000 0.0000 0.0000 0.00939(13) Uani 1 4 d S . .
Cd1 Cd 0.33167(3) 0.0000 0.02826(6) 0.01068(12) Uani 1 2 d S . .
Sb1 Sb 0.20771(2) 0.0000 0.19654(6) 0.00954(11) Uani 1 2 d S . .
Sb2 Sb 0.49775(2) 0.0000 0.31514(5) 0.00988(11) Uani 1 2 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cd Cd -0.8075 1.2024 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Sb1 Ba1 Sb1 87.113(14) 7_556 7_546 ?
Sb1 Ba1 Sb2 171.556(14) 7_556 3_445 ?
Sb1 Ba1 Sb2 93.162(10) 7_546 3_445 ?
Sb1 Ba1 Sb2 93.162(10) 7_556 3_455 ?
Sb1 Ba1 Sb2 171.556(14) 7_546 3_455 ?
Sb2 Ba1 Sb2 85.332(13) 3_445 3_455 ?
Sb1 Ba1 Sb1 87.632(12) 7_556 . ?
Sb1 Ba1 Sb1 87.632(12) 7_546 . ?
Sb2 Ba1 Sb1 83.948(11) 3_445 . ?
Sb2 Ba1 Sb1 83.948(11) 3_455 . ?
Sb1 Ba1 Cd1 48.130(9) 7_556 7_556 ?
Sb1 Ba1 Cd1 103.828(13) 7_546 7_556 ?
Sb2 Ba1 Cd1 139.502(13) 3_445 7_556 ?
Sb2 Ba1 Cd1 82.467(10) 3_455 7_556 ?
Sb1 Ba1 Cd1 132.442(9) . 7_556 ?
Sb1 Ba1 Cd1 103.828(13) 7_556 7_546 ?
Sb1 Ba1 Cd1 48.130(9) 7_546 7_546 ?
Sb2 Ba1 Cd1 82.467(10) 3_445 7_546 ?
Sb2 Ba1 Cd1 139.502(13) 3_455 7_546 ?
Sb1 Ba1 Cd1 132.442(9) . 7_546 ?
Cd1 Ba1 Cd1 82.255(14) 7_556 7_546 ?
Sb1 Ba1 Sb2 143.310(14) 7_556 7_546 ?
Sb1 Ba1 Sb2 84.625(11) 7_546 7_546 ?
Sb2 Ba1 Sb2 45.006(12) 3_445 7_546 ?
Sb2 Ba1 Sb2 100.007(12) 3_455 7_546 ?
Sb1 Ba1 Sb2 127.526(9) . 7_546 ?
Cd1 Ba1 Sb2 99.699(12) 7_556 7_546 ?
Cd1 Ba1 Sb2 46.659(10) 7_546 7_546 ?
Sb1 Ba1 Sb2 84.625(11) 7_556 7_556 ?
Sb1 Ba1 Sb2 143.310(14) 7_546 7_556 ?
Sb2 Ba1 Sb2 100.007(12) 3_445 7_556 ?
Sb2 Ba1 Sb2 45.006(12) 3_455 7_556 ?
Sb1 Ba1 Sb2 127.526(10) . 7_556 ?
Cd1 Ba1 Sb2 46.659(10) 7_556 7_556 ?
Cd1 Ba1 Sb2 99.699(12) 7_546 7_556 ?
Sb2 Ba1 Sb2 81.056(13) 7_546 7_556 ?
Sb1 Ba1 Cd1 46.926(8) 7_556 1_556 ?
Sb1 Ba1 Cd1 46.926(8) 7_546 1_556 ?
Sb2 Ba1 Cd1 136.728(7) 3_445 1_556 ?
Sb2 Ba1 Cd1 136.728(7) 3_455 1_556 ?
Sb1 Ba1 Cd1 106.274(15) . 1_556 ?
Cd1 Ba1 Cd1 59.314(11) 7_556 1_556 ?
Cd1 Ba1 Cd1 59.314(11) 7_546 1_556 ?
Sb2 Ba1 Cd1 105.410(12) 7_546 1_556 ?
Sb2 Ba1 Cd1 105.410(12) 7_556 1_556 ?
Sb1 Ba1 Ba2 122.201(9) 7_556 . ?
Sb1 Ba1 Ba2 122.201(9) 7_546 . ?
Sb2 Ba1 Ba2 51.003(7) 3_445 . ?
Sb2 Ba1 Ba2 51.003(7) 3_455 . ?
Sb1 Ba1 Ba2 50.603(10) . . ?
Cd1 Ba1 Ba2 133.385(8) 7_556 . ?
Cd1 Ba1 Ba2 133.385(9) 7_546 . ?
Sb2 Ba1 Ba2 92.021(10) 7_546 . ?
Sb2 Ba1 Ba2 92.021(10) 7_556 . ?
Cd1 Ba1 Ba2 156.877(12) 1_556 . ?
Sb1 Ba1 Ba1 132.742(8) 7_556 5_556 ?
Sb1 Ba1 Ba1 132.742(8) 7_546 5_556 ?
Sb2 Ba1 Ba1 51.439(8) 3_445 5_556 ?
Sb2 Ba1 Ba1 51.439(8) 3_455 5_556 ?
Sb1 Ba1 Ba1 113.790(14) . 5_556 ?
Cd1 Ba1 Ba1 91.947(11) 7_556 5_556 ?
Cd1 Ba1 Ba1 91.947(11) 7_546 5_556 ?
Sb2 Ba1 Ba1 48.569(8) 7_546 5_556 ?
Sb2 Ba1 Ba1 48.569(8) 7_556 5_556 ?
Cd1 Ba1 Ba1 139.936(15) 1_556 5_556 ?
Ba2 Ba1 Ba1 63.187(8) . 5_556 ?
Sb1 Ba2 Sb1 180.0 . 5 ?
Sb1 Ba2 Sb2 90.676(9) . 7_545 ?
Sb1 Ba2 Sb2 89.324(8) 5 7_545 ?
Sb1 Ba2 Sb2 89.324(8) . 3_455 ?
Sb1 Ba2 Sb2 90.676(8) 5 3_455 ?
Sb2 Ba2 Sb2 180.000(14) 7_545 3_455 ?
Sb1 Ba2 Sb2 90.676(9) . 7 ?
Sb1 Ba2 Sb2 89.324(9) 5 7 ?
Sb2 Ba2 Sb2 89.926(12) 7_545 7 ?
Sb2 Ba2 Sb2 90.074(12) 3_455 7 ?
Sb1 Ba2 Sb2 89.324(9) . 3_445 ?
Sb1 Ba2 Sb2 90.676(9) 5 3_445 ?
Sb2 Ba2 Sb2 90.074(12) 7_545 3_445 ?
Sb2 Ba2 Sb2 89.926(12) 3_455 3_445 ?
Sb2 Ba2 Sb2 180.00(2) 7 3_445 ?
Sb1 Ba2 Cd1 134.040(7) . 3_445 ?
Sb1 Ba2 Cd1 45.959(7) 5 3_445 ?
Sb2 Ba2 Cd1 79.258(9) 7_545 3_445 ?
Sb2 Ba2 Cd1 100.742(9) 3_455 3_445 ?
Sb2 Ba2 Cd1 133.469(9) 7 3_445 ?
Sb2 Ba2 Cd1 46.531(9) 3_445 3_445 ?
Sb1 Ba2 Cd1 45.960(7) . 7 ?
Sb1 Ba2 Cd1 134.041(7) 5 7 ?
Sb2 Ba2 Cd1 100.742(9) 7_545 7 ?
Sb2 Ba2 Cd1 79.258(9) 3_455 7 ?
Sb2 Ba2 Cd1 46.531(9) 7 7 ?
Sb2 Ba2 Cd1 133.469(9) 3_445 7 ?
Cd1 Ba2 Cd1 180.000(9) 3_445 7 ?
Sb1 Ba2 Cd1 134.040(7) . 3_455 ?
Sb1 Ba2 Cd1 45.959(7) 5 3_455 ?
Sb2 Ba2 Cd1 133.469(9) 7_545 3_455 ?
Sb2 Ba2 Cd1 46.531(9) 3_455 3_455 ?
Sb2 Ba2 Cd1 79.258(9) 7 3_455 ?
Sb2 Ba2 Cd1 100.742(9) 3_445 3_455 ?
Cd1 Ba2 Cd1 76.435(11) 3_445 3_455 ?
Cd1 Ba2 Cd1 103.565(11) 7 3_455 ?
Sb1 Ba2 Cd1 45.960(7) . 7_545 ?
Sb1 Ba2 Cd1 134.041(7) 5 7_545 ?
Sb2 Ba2 Cd1 46.531(9) 7_545 7_545 ?
Sb2 Ba2 Cd1 133.469(9) 3_455 7_545 ?
Sb2 Ba2 Cd1 100.742(9) 7 7_545 ?
Sb2 Ba2 Cd1 79.258(9) 3_445 7_545 ?
Cd1 Ba2 Cd1 103.565(11) 3_445 7_545 ?
Cd1 Ba2 Cd1 76.435(11) 7 7_545 ?
Cd1 Ba2 Cd1 180.000(9) 3_455 7_545 ?
Sb1 Ba2 Ba1 54.949(8) . . ?
Sb1 Ba2 Ba1 125.050(8) 5 . ?
Sb2 Ba2 Ba1 125.870(7) 7_545 . ?
Sb2 Ba2 Ba1 54.130(7) 3_455 . ?
Sb2 Ba2 Ba1 125.870(8) 7 . ?
Sb2 Ba2 Ba1 54.130(8) 3_445 . ?
Cd1 Ba2 Ba1 95.712(9) 3_445 . ?
Cd1 Ba2 Ba1 84.288(9) 7 . ?
Cd1 Ba2 Ba1 95.712(8) 3_455 . ?
Cd1 Ba2 Ba1 84.288(8) 7_545 . ?
Sb1 Ba2 Ba1 125.051(8) . 5 ?
Sb1 Ba2 Ba1 54.950(8) 5 5 ?
Sb2 Ba2 Ba1 54.131(7) 7_545 5 ?
Sb2 Ba2 Ba1 125.869(7) 3_455 5 ?
Sb2 Ba2 Ba1 54.131(8) 7 5 ?
Sb2 Ba2 Ba1 125.869(8) 3_445 5 ?
Cd1 Ba2 Ba1 84.288(8) 3_445 5 ?
Cd1 Ba2 Ba1 95.712(8) 7 5 ?
Cd1 Ba2 Ba1 84.288(9) 3_455 5 ?
Cd1 Ba2 Ba1 95.712(9) 7_545 5 ?
Ba1 Ba2 Ba1 180.0 . 5 ?
Sb1 Cd1 Sb1 113.36(2) 7_545 7 ?
Sb1 Cd1 Sb2 113.093(13) 7_545 . ?
Sb1 Cd1 Sb2 113.093(13) 7 . ?
Sb1 Cd1 Sb1 101.947(14) 7_545 . ?
Sb1 Cd1 Sb1 101.947(14) 7 . ?
Sb2 Cd1 Sb1 112.294(19) . . ?
Sb1 Cd1 Ba1 161.675(15) 7_545 7_556 ?
Sb1 Cd1 Ba1 81.375(11) 7 7_556 ?
Sb2 Cd1 Ba1 67.474(11) . 7_556 ?
Sb1 Cd1 Ba1 62.952(10) . 7_556 ?
Sb1 Cd1 Ba1 81.375(11) 7_545 7_546 ?
Sb1 Cd1 Ba1 161.675(15) 7 7_546 ?
Sb2 Cd1 Ba1 67.474(11) . 7_546 ?
Sb1 Cd1 Ba1 62.952(10) . 7_546 ?
Ba1 Cd1 Ba1 82.255(14) 7_556 7_546 ?
Sb1 Cd1 Ba1 62.354(11) 7_545 1_554 ?
Sb1 Cd1 Ba1 62.354(11) 7 1_554 ?
Sb2 Cd1 Ba1 167.923(18) . 1_554 ?
Sb1 Cd1 Ba1 79.783(16) . 1_554 ?
Ba1 Cd1 Ba1 120.685(11) 7_556 1_554 ?
Ba1 Cd1 Ba1 120.685(11) 7_546 1_554 ?
Sb1 Cd1 Ba2 120.148(16) 7_545 3 ?
Sb1 Cd1 Ba2 57.880(10) 7 3 ?
Sb2 Cd1 Ba2 57.956(10) . 3 ?
Sb1 Cd1 Ba2 137.512(8) . 3 ?
Ba1 Cd1 Ba2 76.446(8) 7_556 3 ?
Ba1 Cd1 Ba2 125.412(13) 7_546 3 ?
Ba1 Cd1 Ba2 113.427(11) 1_554 3 ?
Sb1 Cd1 Ba2 57.880(11) 7_545 3_545 ?
Sb1 Cd1 Ba2 120.148(16) 7 3_545 ?
Sb2 Cd1 Ba2 57.956(10) . 3_545 ?
Sb1 Cd1 Ba2 137.512(9) . 3_545 ?
Ba1 Cd1 Ba2 125.412(13) 7_556 3_545 ?
Ba1 Cd1 Ba2 76.446(8) 7_546 3_545 ?
Ba1 Cd1 Ba2 113.427(11) 1_554 3_545 ?
Ba2 Cd1 Ba2 76.435(11) 3 3_545 ?
Cd1 Sb1 Cd1 113.36(2) 7_545 7 ?
Cd1 Sb1 Cd1 78.051(14) 7_545 . ?
Cd1 Sb1 Cd1 78.051(14) 7 . ?
Cd1 Sb1 Ba2 76.161(12) 7_545 . ?
Cd1 Sb1 Ba2 76.161(12) 7 . ?
Cd1 Sb1 Ba2 132.044(17) . . ?
Cd1 Sb1 Ba1 145.227(16) 7_545 7_556 ?
Cd1 Sb1 Ba1 70.719(11) 7 7_556 ?
Cd1 Sb1 Ba1 68.917(12) . 7_556 ?
Ba2 Sb1 Ba1 135.081(7) . 7_556 ?
Cd1 Sb1 Ba1 70.719(11) 7_545 7_546 ?
Cd1 Sb1 Ba1 145.227(16) 7 7_546 ?
Cd1 Sb1 Ba1 68.917(12) . 7_546 ?
Ba2 Sb1 Ba1 135.081(7) . 7_546 ?
Ba1 Sb1 Ba1 87.113(14) 7_556 7_546 ?
Cd1 Sb1 Ba1 114.346(13) 7_545 . ?
Cd1 Sb1 Ba1 114.346(13) 7 . ?
Cd1 Sb1 Ba1 153.509(17) . . ?
Ba2 Sb1 Ba1 74.447(11) . . ?
Ba1 Sb1 Ba1 92.369(11) 7_556 . ?
Ba1 Sb1 Ba1 92.369(11) 7_546 . ?
Sb2 Sb2 Cd1 113.09(2) 5_656 . ?
Sb2 Sb2 Ba2 134.988(6) 5_656 3_545 ?
Cd1 Sb2 Ba2 75.513(10) . 3_545 ?
Sb2 Sb2 Ba2 134.988(6) 5_656 3 ?
Cd1 Sb2 Ba2 75.513(10) . 3 ?
Ba2 Sb2 Ba2 89.925(12) 3_545 3 ?
Sb2 Sb2 Ba1 70.401(13) 5_656 3 ?
Cd1 Sb2 Ba1 137.180(7) . 3 ?
Ba2 Sb2 Ba1 134.165(13) 3_545 3 ?
Ba2 Sb2 Ba1 74.866(9) 3 3 ?
Sb2 Sb2 Ba1 70.401(13) 5_656 3_545 ?
Cd1 Sb2 Ba1 137.180(7) . 3_545 ?
Ba2 Sb2 Ba1 74.866(9) 3_545 3_545 ?
Ba2 Sb2 Ba1 134.165(13) 3 3_545 ?
Ba1 Sb2 Ba1 85.331(13) 3 3_545 ?
Sb2 Sb2 Ba1 64.594(12) 5_656 7_546 ?
Cd1 Sb2 Ba1 65.867(12) . 7_546 ?
Ba2 Sb2 Ba1 82.104(8) 3_545 7_546 ?
Ba2 Sb2 Ba1 141.354(14) 3 7_546 ?
Ba1 Sb2 Ba1 134.995(12) 3 7_546 ?
Ba1 Sb2 Ba1 79.994(11) 3_545 7_546 ?
Sb2 Sb2 Ba1 64.594(12) 5_656 7_556 ?
Cd1 Sb2 Ba1 65.867(12) . 7_556 ?
Ba2 Sb2 Ba1 141.354(14) 3_545 7_556 ?
Ba2 Sb2 Ba1 82.104(8) 3 7_556 ?
Ba1 Sb2 Ba1 79.994(12) 3 7_556 ?
Ba1 Sb2 Ba1 134.995(12) 3_545 7_556 ?
Ba1 Sb2 Ba1 81.057(12) 7_546 7_556 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ba1 Sb1 3.5319(4) 7_556 ?
Ba1 Sb1 3.5319(4) 7_546 ?
Ba1 Sb2 3.5911(4) 3_445 ?
Ba1 Sb2 3.5911(4) 3_455 ?
Ba1 Sb1 3.6351(6) . ?
Ba1 Cd1 3.7002(5) 7_556 ?
Ba1 Cd1 3.7002(5) 7_546 ?
Ba1 Sb2 3.7453(5) 7_546 ?
Ba1 Sb2 3.7453(5) 7_556 ?
Ba1 Cd1 3.7635(6) 1_556 ?
Ba1 Ba2 4.2778(5) . ?
Ba1 Ba1 4.7168(8) 5_556 ?
Ba2 Sb1 3.4314(5) . ?
Ba2 Sb1 3.4314(5) 5 ?
Ba2 Sb2 3.4441(4) 7_545 ?
Ba2 Sb2 3.4441(4) 3_455 ?
Ba2 Sb2 3.4441(4) 7 ?
Ba2 Sb2 3.4441(4) 3_445 ?
Ba2 Cd1 3.9340(4) 3_445 ?
Ba2 Cd1 3.9340(4) 7 ?
Ba2 Cd1 3.9340(4) 3_455 ?
Ba2 Cd1 3.9340(4) 7_545 ?
Ba2 Ba1 4.2778(5) 5 ?
Cd1 Sb1 2.9125(4) 7_545 ?
Cd1 Sb1 2.9125(4) 7 ?
Cd1 Sb2 2.9488(6) . ?
Cd1 Sb1 2.9531(6) . ?
Cd1 Ba1 3.7002(5) 7_556 ?
Cd1 Ba1 3.7002(5) 7_546 ?
Cd1 Ba1 3.7635(6) 1_554 ?
Cd1 Ba2 3.9340(4) 3 ?
Cd1 Ba2 3.9340(4) 3_545 ?
Sb1 Cd1 2.9125(4) 7_545 ?
Sb1 Cd1 2.9125(4) 7 ?
Sb1 Ba1 3.5319(4) 7_556 ?
Sb1 Ba1 3.5319(4) 7_546 ?
Sb2 Sb2 2.8114(8) 5_656 ?
Sb2 Ba2 3.4441(4) 3_545 ?
Sb2 Ba2 3.4441(4) 3 ?
Sb2 Ba1 3.5911(4) 3 ?
Sb2 Ba1 3.5911(4) 3_545 ?
Sb2 Ba1 3.7452(5) 7_546 ?
Sb2 Ba1 3.7452(5) 7_556 ?
